1 Missouri University of Science and Technology Scholars' Mine Materials Science and Engineering Faculty Research & Creative Works Materials Science and Engineering Alloy Recovery and Control in Steel Melting Kent D. Peaslee Missouri University of Science and Technology Darryl S. Webber Semen Naumovich Lekakh Missouri University of Science and Technology, Bradley Randall Follow this and additional works at: Part of the Materials Science and Engineering Commons Recommended Citation K. D. Peaslee et al., "Alloy Recovery and Control in Steel Melting," Proceedings of the SFSA Technical and Operating Conference, Steel Founders' Society of America (SFSA), Jan This Article - Conference proceedings is brought to you for free and open access by Scholars' Mine. It has been accepted for inclusion in Materials Science and Engineering Faculty Research & Creative Works by an authorized administrator of Scholars' Mine. This work is protected by U. S. Copyright Law. Unauthorized use including reproduction for redistribution requires the permission of the copyright holder. For more information, please contact
2 Alloy Recovery and Control in Steel Melting Kent D. Peaslee, Darryl S. Webber, Simon Lekakh and Bradley Randall Department of Materials Science and Engineering University of Missouri-Rolla Rolla, MO Abstract Alloy recovery plays an important role in steel melting economics because the cost of alloying additives such as ferroalloys and pure non-ferrous metals is significantly higher than the cost of steel scrap. Recovery of alloying additives also influences the reproducibility of steel properties from heat to heat. This paper reviews alloy recovery and final chemistry distributions at seven steel foundries and preliminary laboratory studies of alloy dissolution in ladles. Melting and alloy practices were observed for several plant trial heats in each of the foundries. Alloying and chemistry data were collected for an additional heats at each plant. The recovery of alloying additives depends on the type of furnace and individual foundry practices. EAF operations had greater variations in final chemistry performance than induction furnace operations. Laboratory experiments showed that there is a potential for increased alloy recovery and control through argon stirring with a porous plug. Argon stirring decreased mixing time by 50% and decreased the local variation in steel composition. Introduction One of the highest costs in a melting operation is alloy additions. Therefore, if a foundry can have a better understanding of the factors that determine alloy recovery and improve control of the final chemistry, significant costs can be saved while producing more consistent quality steel castings. Alloy control implies that a foundry has the ability to meet the chemistry requirements for a given grade consistently. As illustrated in Figure 1, the typical foundry practice is to aim well above the minimum alloy requirement, usually at or just slightly above the mid-specification range, avoiding off-specification castings. As control is improved, alloy savings can be realized by targeting a much tighter internal chemistry specification at the lower end of the alloy requirement (see Figure 1). Both alloy recovery and melt practice play key roles in foundries being able to utilize alloy control. Recovery of alloying additives is important not only from an economical standpoint but also from the standpoint of making high quality products with highly reproducible mechanical properties. In spite of smaller absolute amount of additives, in many cases the total relative expenses can be significant because frequently used elements like Cr, Ni and Mo can cost tens to hundreds of times more than steel scrap. Recovery of additives depends on a vast spectrum of parameters, summarized in three groups: Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
3 1. Type of additives (concentration of the alloying elements and their chemical activity, in particular, affinity to oxygen, density, size and shape of particles, concentration of impurities); 2. Methods of alloying (in furnace or ladle, special injection methods, such as wire injection, in stream or in the mold treatments, intensifiers of dissolution by mixing); 3. Melting techniques (type and size of melting furnaces, slag composition, condition, and quantity, temperature of melt, melting period). Controlled alloying Frequency Typical alloying Alloy savings Specification range % alloy Figure 1. Savings from controlled alloying in place of the typical alloying practice of many foundries Alloy recovery in industrial operations is affected by many factors. Oxidation of the alloy is usually the primary cause of poor or erratic recovery. Research suggests that ferroalloy recovery is a function of the dissolution rate of the alloy, density of the alloy, and dissolved oxygen in the liquid steel (for nitride forming alloys, dissolved nitrogen must also be included). 1 It was found that increasing the dissolved oxygen in the steel lowered the alloy recovery and decreased the dissolution rate of alloys with melting points greater than steel. The reduction in dissolution rate was attributed to the possible formation of a refractory oxide on the alloy surface. Important sources of oxygen are furnace slag and air contact (slag carryover and air entrainment during tapping). 2 Other sources of oxygen include slag remaining in the furnace (or ladle) from previous heats, oxygen dissolved in the metal, air carried into the melt by alloy additions, and from refractory-metal interactions. In order to transfer alloying elements to the molten steel bath, it is first necessary to immerse the ferroalloy into the metal. Upon addition, a steel shell is frozen on the surface of the alloy. Heat transferred from the molten bath remelts this shell back to the original alloy surface. Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
4 Convective heat transfer, which is a function of bath stirring and superheat, governs shell melting. Several physical and chemical properties of alloy additions affect how the element is incorporated into the steel melt. Melting point is the primary factor in dissolution rate, while other important properties include density, thermal conductivity, specific heat, and enthalpy of mixing. Density determines whether the addition will float (ferrosilicon), sink (ferromanganese) or be entrained within the melt (ferrochromium). Thermal conductivity, along with specific heat and density, determines the thickness of the steel shell, which forms on the cold addition. Finally, a strong exothermic reaction between the alloy and steel (enthalpy of mixing) can substantially reduce the assimilation time (75% ferrosilicon). Minimizing alloy size improves dissolution rate, which is contrary to historical practice where large lumpy ferroalloys were employed to aid in penetrating the slag layer. Unfortunately, small size means more surface area on which to transport undesirable gases and moisture, plus, small alloy size increases dust losses and incurs handling difficulties. Lee et al. determined that the optimum size for bulk materials is between 3 and 20 mm in diameter. 3 Wire and powder injection are both means of overcoming limitations imposed by fine alloy size. Efficient steelmaking processes rely on the motion of molten steel to: dissolve alloys, float inclusions, and eliminate chemical and temperature inhomogeneities. Natural forces can induce steel motion, e.g. convection due to temperature gradient or energy of the falling stream during tap. Natural convection is relatively slow; while tap induced motion is time limited. In contrast, external forces, like induction stirring in induction furnaces, or gas injection through a lance, plug, or tuyere can create significantly more intense motion. Gas injection via lances and porous plugs is the predominant method of stirring used in wrought steel production. Wrought steel producers typically do not add alloys to the melting furnace and make sixty to ninety percent of bulk alloy additions to the ladle during tapping of the steel. However, there is a trend in the wrought industry towards making more additions at the ladle metallurgy station/ladle furnace or even at the tundish using specialty wire products 4,5. By, moving chemical correction from the melting furnace to the ladle, the modern steel mini-mill practice of minimizing time and energy consumption in the EAF has been achieved. Of course, the effectiveness of the above described alloying methods depends on ladle volume. Thus, not all of these techniques can be effectively used in foundries which operate with multiple smaller ladles. Additional research will be necessary for adaptation of these methods to foundry practice. The main aims of this research were to evaluate the recovery of alloying additives in foundry practices and investigate controlled alloying by argon stirring in small-scale ladle. Methodology Melting observation and statistical data were used for analysis of alloying additive recovery and steel chemistry distribution in industrial practices. Seven foundries equipped with induction furnaces (IF) and electric arc furnaces (EAF) were observed. All foundries are Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
5 designated by a letter from A to G to identify the facility while maintaining confidentiality. In addition, lab experiments were performed to determine the effects of ladle stirring on alloy dissolution. Steel foundry observations. Three to five trial heats were melted and observed in each foundry and the following data was recorded: Melting procedure and power-on time Weight and composition of charge materials Weight, composition of additives, and alloying procedure Steel chemistry before and after alloying. All of the foundries weighed charge materials and tested the chemistry analysis before and after the alloy additions. However, some foundries weighed additives more precisely than others. Statistical data. At each foundry, an additional 20 to 155 heats were studied by recording the charge weight and compositions, preliminary and final steel chemistry, and the weight of additives from statistical data available at the plant (charge sheets, heat logs, cast logs, computer databases, etc.). Experimental procedure. Laboratory experiments are being conducted at UMR to examine the role of gas stirring in alloy dissolution. One hundred pound heats of steel are induction melted and poured into a ladle where a bulk alloy addition is made. Consecutive timed samples are then taken for chemical analysis. The ladle is equipped with a porous plug in the bottom for the introduction of argon gas for stirring. This paper will discuss some of the initial tests. Induction furnaces (IF) Steel Foundry Melting Study Four steel foundries with different capacity induction furnaces are included in this study. All of the furnaces had medium frequency power supplies and were lined with alumina based (alumina spinel) refractory. Heats were batch melted and often utilized a liquid heel resulting from excess steel being returned from the previous heat instead of pigging. Foundries A, B, and F typically melt 8 to 12 hours per day with the furnaces setting idle (and cold) during the off-shifts. Foundry G melts by induction furnace occasionally and on those days typically melts only one heat per day in a furnace. The variety in melting schedules resulted in wide differences in the percentage of heats melted in furnaces with hot linings (ranged from 0% to greater than 80%). Table 1 compares the furnace capacity and transformers at each of the plants. The following summarizes the alloy recovery findings at each of the induction furnace melting facilities. Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
6 Table 1. Inductions furnace capacity and characteristics Foundry Capacity, lb Power supply, KW Lining Steel A Alumina spinel Carbon, alloy B Alumina spinel Carbon, alloy F Alumina spinel Alumina spinel Carbon, alloy, Stainless G Alumina spinel Carbon, alloy Foundry A. Melting and alloying of three heats of low carbon steel were observed. The typical melting practice was to charge some carbon with the scrap. Typically, ferrosilicon (75% Si) and electrolytic manganese were added to the furnace at o F after taking the preliminary chemistry test. Because the surface was not deslagged prior to adding the alloys, some of the addition went into the metal and some was lost to the slag. Additional carbon was typically added on a clean melt surface at higher temperatures after deslagging with the assistance of slag coagulant. Aluminum and other deoxidizers were added directly in ladle during tapping. All additives were weighed. The range of recoveries for the various alloying elements in the trial heats and from statistical data for 155 previous heats are provided in Table 2. Recoveries were lower for elements when added to the charge because of the greater potential for oxidation during the melting process. The recovery values for and Si in the melt were lower during the historical heats (155 heats) than during the observation period most likely because of additional oxidation from the surface slag. Table 2. Recovery (%) of alloying elements in IF Foundry A Method of alloying C Si In Charge In Melt In melt (statistics of 155 heats) Table 3 compares the chemistry change in the slag during one of the trial heats. The large O increase in the slag after alloying indicates the losses of alloy directly to the slag during the alloying process. As expected, the ladle slag had higher levels of aluminum and titanium oxides. Table 3. Slag compositions, weight % (Foundry A) Slag SiO 2 Al 2 O 3 Fe 2 O 3 MgO CaO Na 2 O K 2 O TiO 2 O Cr 2 O 3 IF-primary IF-after alloying Ladle-after Al+FeTi Statistical variations in the final and Si contents in low carbon steel were evaluated by calculating the difference between the final chemistry (C f ) and aim chemistry (C aim ). Final chemistry distributions are shown in Figure 2 and the statistical parameters (median - M and Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
7 standard deviation -SD) for the data are displayed in Table 4. Although the specification range (SR) for alloying elements in steel castings is typically different for each plant and only an aim range, the ratio of SR/SD provides an indication of the capability each plant has to control alloy levels with present practices. From a statistical point of view, a SR/SD ratio of 4.0 indicates that 95,5% of the heats would be within the specification range based upon a normal data distribution. Statistically, the C is in control (SR/SD=5) but the Si and show much greater variation with the Si skewed under the aim and with a bimodal distribution. Table 4. Final steel chemistry (wt%) for 155 heats produced in IF (Foundry A) Parameters C Si Aim Median (M) Standard deviation (SD) Specification Range (SR) SR/SD Frequency, % C Si Element variation Figure 2. Variations of steel final concentration (IF, Foundry A) Foundry B. The melt shop at Foundry B operated two 9500 lb capacity induction furnaces simultaneously from one 4500 KW energy supply unit. The high specific value of energy input (near 1000 KW/ton) gave short melting times and intensive stirring of the liquid steel. Once the charge was completely melted, a preliminary chemical analysis sample was taken and the primary slag removed with assistance of coagulant. Alloys were added to a clean melt surface at o F under full power. Statistical values of recovery of from ferromanganese, Cr from low carbon ferrochrome, Mo from ferromolybdenum, and pure Ni are given in Table 5. Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
8 Table 5. Recovery (%) of alloying elements in 24 IF heats at Foundry B Cr Mo Ni Recovery in melt Final chemistry distributions and the statistical parameters for 24 IF alloy heats are illustrated in Figure 3 and Table 6. Note that this foundry is capable of tighter chemistry controls with present melting practices. Table 6. Statistics of final steel chemistry (wt%) produced in IF for 24 heats (Foundry B) Cr Ni Mo Aim M SD Specification Range SR/SD Frequency, % NI Mo Cr Element variation, % Figure 3. Variations of steel final concentration (IF, Foundry B) Foundry F. Foundry F melted highly alloyed stainless steels in induction furnaces during the period of observation. Alloy scrap and revert were charged in the furnace along with a part of the low carbon ferrochromium. After melting the charge and taking a preliminary chemical analysis, the primary slag was removed with coagulant and the metal heated to 2850 o F. Low carbon ferrochromium, nickel, and electrolytic manganese were weighed and added to the open melt surface under full power. The range of variation in the Cr, Ni,, and Mo recovery during the four observed heats are summarized in Table 7. Table 7. Recovery of alloying elements in four IF heats (stainless steel at Foundry F), % Method of alloying Cr Mo Ni In Melt Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
9 Electric Arc Furnaces (EAF) Four foundries equipped with EAFs having capacities ranging from 2.5 to 15 ton were observed to study alloy additive recovery and control. These foundries used both acid and basic melting practices and linings (see Table 8). Although some of the foundries had AODs, only non-aod heats were analyzed in this paper. Table 8. EAF furnaces observed in plant trials Foundry #EAF Typical heat, lb Lining Steel C Magnesia Carbon, alloy, stainless D 1, Silica Carbon, low alloy E 1, 2, , 8500, 9400 Silica Carbon, low alloy G 2, , 8500 Magnesia Carbon, low alloy Foundry C. Three heats of low and medium carbon steel were studied with different melting practices including one heat with a cold lining, one heat with a heel and hot lining, and one heat with a pour-back on solid charge and hot lining. During these heats, 75 lb of carbon and lb of ferrosilicon (75% Si) were added to the furnace with the scrap charge. After melting, oxygen boiling, preliminary chemical testing, and a CaCO 3 addition, chemistry correction was accomplished by adding ferromanganese and ferrosilicon. The recovery from this addition may have been affected by the significant amount of slag in the furnace. Carbon correction was made by a combination of pig iron and 1-3 minutes of dipping the graphite electrodes. Typical changes in the steel composition during the heat are summarized in Table 9. Table 9. Changing chemistry (wt %) during melting steel in EAF Operation C Si P S Melt-in preliminary test After oxygen blow After CaCO 3, FeSi, Fe, and C additions Statistical variations of carbon, silicon, and manganese final concentrations are summarized in Figure 4 and Table 10. This foundry will require some change in practice to improve alloy control based on the relatively low SR/SD values. However, the is skewed to the high side and the aim could be lowered to save alloy costs. Table 10. Statistics for final steel chemistry (wt %) produced in 59 EAF heats (Foundry C) C Si Aim M SD Specification Range SR/SD Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
10 Frequency, % C Si Element variations, % Figure 4. Variations of steel final concentration (EAF, Foundry C) Foundry D. Four EAF trial heats were observed for this study. All were melted in a silica lined furnace with an acid slag practice. All materials were weighed before charging with no ferroalloys placed in the charge. Once the scrap is melted, a chemical sample is taken and the bath blown with oxygen for five to ten minutes. The ferroalloys are added once the temperature is at o F. The recovery of and Si, as well as the statistical study of 21 heats is summarized in Table 11 and Figure 5. Both the and Si curves are skewed to the high side of the range. There are opportunities to save alloys through alloy practice changes. Table 11. Statistics of final steel chemistry produced in EAF for 21 heats (Foundry D) Si Recovery, % Aim M SD Specification Range SR/SD Foundry E. This foundry operates three EAFs with silica lining. EAF #1 and #2 used oxyfuel burners for accelerated preheating and melting of the solid charge with total heat times of less than 60 minutes. Statistical data for Si and recovery for manganese and silicon additions in the EAF are summarized in Table 12. Distributions of alloying element compositions in the final melt for Furnace #3 were closest to the aim of the three furnaces and showed the least amount of variation as illustrated in Figure 6. Statistical parameters for the three furnaces are summarized in Table 13. Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
11 Frequency, % Si Element variation, % Figure 5. Variations of steel final concentration (EAF, Foundry D) Table 12. Statistics of and Si recovery (%) in EAF for 150 heats (Foundry E) Furnace Practice Si #1 Fe & FeSi in EAF #2 Fe & FeSi in EAF #3 Fe & FeSi in EAF + FeSiBa in ladle Table 13. Statistics of final steel chemistry (wt %) produced in 150 EAF heats (Foundry E) Si EAF #1 EAR#2 EAF #3 EAF #1 EAF#2 EAF #3 Aim M SD Specification Range SR/SD Frequency, % Si Element variation, % Figure 6. Variations of steel final concentration (EAF #3, Foundry E) Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
12 Foundry G. Statistical data distribution for the final and Si compositions in 37 heats melted in #2 EAF are summarized in Table 14. This furnace used a magnesia furnace and basic melt practice. Table 14. Statistics of final steel chemistry (wt %) produced in 37 EAF heats (Foundry G) Si M SD Specification Range SR/SD Preliminary Dissolution and Stirring Work Work has started at UMR to examine the factors that affect dissolution rate. Results from some of the preliminary melts are plotted in Figure 8. In this series of experiments, a single addition of low carbon ferromanganese (raise by 0.30%) was added to 100 lbs of 0.80% C steel in a special ladle with a porous plug mounted in the bottom. Two factors were varied in this series: ferroalloy size (0.79 inch diameter versus 1.18 inch diameter) and argon flow rate. Preliminary results suggest that alloy particle size is a more critical factor in dissolution rate than argon stirring. Future research will determine the factors that are most important to alloy control for foundries Change: Weight % in scfm Argon 0.79 in scfm Argon 0.79in - 0 scfm Argon 1.18 in scfm Argon 1.18 in scfm Argon Time From Addition - Seconds Figure 7. Change in Manganese Weight Percent with Time Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
13 Summary This study of seven steel foundries showed that there is a vast variety of factors which influence the recovery of ferroalloys and the ability to tightly control final chemical composition. Table 15 shows the wide variation in recoveries and alloy control capabilities between six of the foundries studied in this paper, induction furnace studies at UMR, and UMR trials at a LMF in a mini-mill. The intensive mixing in induction furnaces provides better homogeneity of alloying elements in final melt. The best industrial results were achieved in Foundry B, where recoveries of, Cr, Ni, and Mo were high and the chemistry control was tighter. The laboratory results at UMR were slightly better than industrial operations due to the improved recovery in the ladle. Some of the factors observed in this study that affected alloy recovery and control (negative and positive) in induction furnaces included: Oxidizing conditions (melting in air, additives with charge, and slag on surface during alloying) Induction stirring after alloy addition Time of addition (charge, in furnace, or in ladle) Accuracy of weights and additions Alloying in EAF furnaces was generally less accurate than in induction furnaces resulting in chemistry distributions with more scatter (see Figure 8). Figure 8 shows the improvement in recovery and control that can occur when alloys are added in the ladle. Some of the factors observed in this study that affected alloy recovery and control (negative and positive) in EAFs included: Lack of intense stirring resulting in less homogeneous chemistry More slag Time of addition (with charge-low recovery, in furnace, or in ladle-high recovery) Accuracy of weights and additions Dipping electrodes is extremely expensive method of adding carbon Figure 8 shows the wide variation in chemistry control that occurs in foundries today. There are many opportunities for improvements that will save alloying costs as well as providing customers with steel castings that are more consistent in properties. Table 15. Recovery and variation of in different melting practices IF EAF % A B UMR C E D G LMF Recovery SD SD/M SR/SD NA Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
14 Frequency, % EAF - Foundry E IF - Foundry B EAF - Foundry D EAF - Foundry C IF - Foundry A EAF - Foundry G variation, % Figure 8. Variation of manganese concentration in steel melting in different foundries. Acknowledgments The authors wish to thank the Steel Founders Society of America and the member companies that have provided support for this work. This work is supported by the U. S. Department of Energy Assistance Award No. DE-FC36-04GO14230, Energy Saving Melting and Revert Reduction Technology ( Energy SMARRT ) Program, Subtask No Such support does not constitute an endorsement by DOE of the views expressed in the article. References 1 Sismanis, P.G.; Argyropoulos, S. A.; The Effect of Oxygen on the Recovery and Dissolution of Ferroalloys Proceedings of the 69 th Steelmaking Conference, Vol. 69 (1986), pp Tanaka, M.; Mazumdar, D.; Guthrie, R.I.L.; Motions of Alloying Additions During Furnace Tapping in Steelmaking Processing Operations Metallurgical Transactions B: Process Metallurgy (1993), Vol. 24B, No.4, p Lee, Y; Berg, H.; Jensen, B.; Sandberg, J.; Ferroalloy Size in Steelmaking 54 th Electric Furnace Conference Proceedings, Iron and Steel Society, Vol. 54 (1996), pp Berg, H.; Laux, H.; Johansen, S. T.; Klevan, O. S.; Flow Pattern and Alloy Dissolution During Tapping of Steel Furnaces Ironmaking and Steelmaking, Vol. 26 (1999), No. 2, pp Schade, J.; Argyropoulus, S. A.; Mclean, A.; Cored-Wire Microexothermic Alloys for Tundish Metallurgy Transactions of the Iron and Steel Society, Vol. 12 (1991), pp Alloy Recovery and Control in Steel Melting Proceedings of 58 th SFSA T&O Conf.
Final Technical Report Project Title: Melting Efficiency Improvement Award Number: DE-FC36-04GO14230 Project Period: (January 2004 June 2012) Principal Investigator: Kent Peaslee, 573-341-4714, firstname.lastname@example.org
Missouri University of Science and Technology Scholars' Mine Materials Science and Engineering Faculty Research & Creative Works Materials Science and Engineering 12-1-28 Using Automated Inclusion Analysis
U.P.B. Sci. Bull., Series B, Vol. 75, Iss. 2, 2013 ISSN 1454-2331 REFINING STEELS PRODUCED IN ELECTRIC ARC FURNACE Valentin MINCU 1, Nicolae CONSTANTIN 2 Characteristics and properties of cast and forged
Thermochemistry and Kinetics of Iron Melt Treatment Simon N. Lekakh *, David G. C. Robertson * and Carl R. Loper Jr. ** * University of Missouri Rolla, ** University of Wisconsin-Milwaukee, U.S.A. Abstract
EAF REFRACTORY PERFORMANCE AT PACIFIC STEEL NEW ZEALAND Don Sanford Product Manager Refractories Chemiplas, New Zealand Ltd Level 2, 42 Upper Queen Street Auckland, New Zealand DonS@chemiplas.co.nz Brian
Materials engineering Iron and steel making Metals: rarely exist in pure state mostly in ores Ore: Metallic and other compounds, mostly oxides Metallic content: Iron ores: 30-70% Fe Copper ores: 0.1-0.8
Effect of Charge Materials on Slag Formation in Ductile Iron Melts C. Labrecque, M. Gagné and E. Planque Rio Tinto Iron & Titanium Inc. Sorel-Tracy, Quebec, Canada ABSTRACT The formation of an oxide slag
Lecture 14 Modern trends in BOF steelmaking Contents: Post combustion Technology of post combustion Potential post combustion issues Slag splashing What is required for slag splashing Liquidus temperature
Lecture 12 Converter Steelmaking Practice & combined blowing Contents: Refining of hot metal Composition and temperature during the blow Physico-chemical interactions Developments in Top blown steelmaking
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Manganese concentrate usage in steelmaking To cite this article: O I Nokhrina and I D Rozhihina 2015 IOP Conf. Ser.: Mater. Sci.
INTRODUCTION PROCESS TECHNOLOGY CONFERENCE PROCEEDINGS VOLUME 11 ATLANTA, GA 1992 Ultra-Refining Processes for Specialty Steelmaking A PUBLICATION OFTHE IRON AND STEEL SOCIETY Reprinted from 11th Process
EAF Technology and process In the last 100 years,the EAF technology has evolved to meet the demands of higher productivity, improved quality of product and flexibility of metallic inputs. The product mix
Ferro-Niobium Market Trend and Alloying Techniques Dr Jitendra Patel 1,2 Director - International Metallurgy Ltd- UK CBMM Technology Suisse S.A. - Switzerland BACKGROUND Niobium does not occur in nature
Journal of Minerals & Materials Characterization & Engineering, Vol. 1, No.2, pp69-78, 2002 Printed in the USA. All rights reserved RECYCLING PRACTICES OF SPENT MgO-C REFRACTORIES Kyei-Sing Kwong and James
ELECTRIC INDUCTION FURNACE The electric induction furnace is a type of melting furnace that uses electric currents to melt metal. Induction furnaces are ideal for melting and alloying a wide variety of
EFFECT OF CHROME ORE QUALITY ON FERROCHROME PRODUCTION EFFICIENCY M.H. Farjadi and J. Azari Faryab Mining Company, 54 Sohrevardi Ave. Tehran, Iran. E-mail: email@example.com and firstname.lastname@example.org
Twinjection Technology Improves Hot Metal Desulphurisation at Corus Scunthorpe Works Dr. Robert Robey, Process Metallurgist, Mark Whitehead, Manager - Technical Sales, SMS Mevac UK Limited, Winsford, UK;
Manufacture of Iron & Steel Prepared By: John Cawley Presentation Objectives Identify the basic steps in the production of steel. Identify the properties and uses of iron ore and pig iron. Differentiate
Chapter 2 Electric Arc Furnace as Thermoenergetical Unit 2.1 Thermal Performance of Furnace: Terminology and Designations There are different forms of energy. Heat is one of them. Heat is a form of energy
VŠB - Technical University of Ostrava Faculty of Metallurgy and Materials Engineering Steel Casting Foundry (study supports) doc. Ing. Libor Čamek, Ph.D. Ostrava 2016 1. Basic parameters of electric arc
HIGHVELD STEEL PROSPECTUS IRON MAKING PLANT 1 January 2018 IRON MAKING PLANT 1 EXECUTIVE SUMMARY Highveld Steel and Vanadium was founded in 1960 with the objective of building a unique plant with the ability
University of Wollongong Research Online Faculty of Engineering - Papers (Archive) Faculty of Engineering and Information Sciences 2012 Why do we need new inclusion experimental techniques? Neslihan Dogan
Electric Arc Furnace Simulation User Guide Version 1 1 Introduction and Disclaimer...2 2 Introduction to Electric Arc Furnace Steelmaking...2 2.1 Basic Concepts... 2 2.2 Heating and Melting... 2 2.3 Other
Fast and reliable temperature measurement at end of melting cycle in EAF CoreTemp product description Page 1 Summary In modern mini-mill setups, the EAF is considered primarily as a melting unit. Under
IRONMAKING and STEELMAKING THEORY AND PRACTICE Ahindra Ghosh Amit Chatterjee IRONMAKING AND STEELMAKING IRONMAKING AND STEELMAKING Theory and Practice AHINDRA GHOSH Formerly Professor Materials and Metallurgical
Acta Metall. Slovaca Conf. 189 THE INFLUENCE OF BRIQUETTED SYNTHETIC SLAGS ON STEEL REFINING IN LADLE Ladislav Socha 1)*, Jiří Bažan 1), Pavel Machovčák 2), Aleš Opler 2), Petr Styrnal 3) 1) VŠB Technical
Rolling Process Metallurgical Aspects Material Specifications and Chemistries Standard Mill Practices Miscellaneous Tables & Data Elastic Section Modulus Plastic Section Modulus Moment of Inertia SI Conversion
DEVELOPMENT OF ULTRA-CLEAN AND LOW-COST PROCESS FOR GALVANIZED STEEL BY LADLE FURNACE BY CHI-WEI TAI*, CHUNG-YI LI**, TONG-FA YEH*** SYNOPSIS: The standard process of high quality galvanized steel (GI)
ABSTRACT MASS AND HEAT BALANCE OF STEELMAKING IN BOF AS COMPARED TO EAF PROCESSES M.M.LOTFY 1, H.A.AHMED 2 AND F.A.ELREFAIE 3 Mass and energy balance equations are applied on top blowing BOF and EAF steelmaking
Vacuum Cap Furnaces Vacuum Cap Furnace New vacuum degassing and controlled atmosphere melting technology from Consarc. Consarc, an Inductotherm Group Company, has developed a new range of induction melting
Institut für Eisenhüttenkunde Rheinisch-Westfälische Technische Hochschule Aachen Advanced Master Course Process Technology of Metals (Part: Ferrous Process Metallurgy) Prof. Dr.-Ing. D. Senk 16-04-2010
jmmce.org Journal of Minerals & Materials Characterization & Engineering, Vol. 11, No.1, pp.1-2, 212 Printed in the USA. All rights reserved Parameters Affecting the Production of High Carbon Ferromanganese
ALUMINUM POWDER METALLURGY Increased demand for light weight components, primarily driven by the need to reduce energy consumption in a variety of societal and structural components, has led to increased
IOP Conference Series: Materials Science and Engineering OPEN ACCESS Researches on the production of self-reducing briquettes from waste containing iron and carbon To cite this article: E Ardelean et al
Brochure The is a fully integrated, linear programming software package that will optimize site specific melting economics. Your customized solution could include the following: Least Cost Charge Design
Production of Steel by the Bessemer Process By E. F. Ketterer* THE pneumatic steelmaking process invented by William Kelly and Henry Bessemer, and commonly known as the bessemer process, has been in use
HOOK CRACK IN ELECTRIC RESISTANCE WELDED LINE PIPE STEEL BY SIMA AMINORROAYA *, HOSSEIN EDRIS **, MEHRDAD FATAHI *** SYNOPSIS: One of the production methods for API line pipe steel is electric resistance
FUNDAMENTALS OF EAF AND LADLE SLAGS AND LADLE REFINING PRINCIPLES By Eugene Pretorius Baker Refractories Epretorius@bakerref.com 1 I) Introduction TABLE OF CONTENTS II) Introduction to slag fundamentals
Thermodynamic database of P 2 O 5 -containing oxide system for De-P process in steelmaking *In-Ho JUNG, Pierre HUDON, Wan-Yi KIM, Marie-Aline VAN ENDE, Miftaur RAHMAN, Gabriel Garcia CURIEL, Elmira Moosavi
Metal Powder - the Raw Material of Future Production BY GÜNTER BUSCH* SYNOPSIS Alongside Mobile Internet, Cloud Computing, Robotics, Energy Storage and Autonomous Vehicles, Additive Manufacturing is one
Higher cost and resource efficiencies during stainless steelmaking in an EAF Victor Yuardi Risonarta, Markus Kirschen, Thomas Echterhof, Hans Peter Jung, Stefan Lenz, Christof Beiler and Herbert Pfeifer
8A th Successful Middle East Model Iron and of Steel Cost Conference Reduction in the Melt Shop A successful model of cost reduction in the Middle East Iron and Steel Conference Atlantis, The Palm, Dubai,
STEEL FOUNDERS' SOCIETY OF AMERICA TECHNICAL SERVICE REPORT #124 ANALYSIS OF DEFECTS OF THE BORED SURFACE OF SIX 1025 CARBON STEEL CASTINGS Published by the STEEL FOUNDERS' SOCIETY OF AMERICA Malcolm Blair
Southern African Pyrometallurgy 2006, Edited by R.T. Jones, South African Institute of Mining and Metallurgy, Johannesburg, 5-8 March 2006 Laboratory Investigations of the Electrical Resistivity of Cokes
Tool 2016, Bratislava, October 5 th 2016 Melting and casting technologies for the production of tool steels Dr. Harald Holzgruber, CEO DI Alexander Scheriau, CSO Global Alloy Tool Steel Products 2015 [
Southern African Pyrometallurgy 2011, Edited by R.T. Jones & P. den Hoed, Southern African Institute of Mining and Metallurgy, Johannesburg, 6 9 March 2011 The history and development of the pyrometallurgical
Arch. Metall. Mater. 62 (2017), 2, 885-889 DOI: 10.1515/amm-2017-0130 J. FALKUS* # AN EVALUATION OF THE STABILITY OF MOULD FLUX PROPERTIES IN THE PROCESS OF CONTINUOUS STEEL CASTING This paper presents
DRI Direct Reduced Iron What is DRI? Sponge iron/dri has gained great prominence in world as a substitute of steel scrap (partially) in steel making in electric arc furnace and in induction furnace. Direct
ERIKSSON, J and BJÖRKMAN, B. MgO modification of slag from stainless steelmaking. VII International Conference on Molten Slags Fluxes and Salts, The South African Institute of Mining and Metallurgy, 2004.
Fused Magnesia Trends & Global Outlook Asım Bilge MagForum 2016, Vienna Kümaş Manyezit San. A.Ş. Contents Fused Magnesia Global FM Market, Demand and Prices Effects of Global Economy Issues Kümaş FM Production
Development of the process for production of vanadium rich slag and low silicon pig iron from vanadium bearing titaniferous magnetites of Masanikere at VISL, Bhadravati By THE STAFF OF NML fr VISL, Presented
Copyright(c)JCPDS-International Centre for Diffraction Data 2001,Advances in X-ray Analysis,Vol.44 398 XRF S ROLE IN THE PRODUCTION OF MAGNESIUM METAL BY THE MAGNETHERMIC METHOD H. L. Baker Northwest Alloys,
76 BENEFIT OF GAS PURGING IN BOF AND EAF WITH A FOCUS ON MATERIAL EFFICIENCY AND EMISSION REDUCTION. Thomas Kollmann, Marcus Kirschen, Christoph Jandl, Karl-Michael Zettl RHI AG, Vienna Abstract In highly
Preface... xi Chapter 1. Metallurgical Thermochemistry... 1 1.1. Introduction... 1 1.2. Quantities characterizing the state of a system and its evolution... 3 1.2.1. The types of operations... 3 1.2.2.
CHAPTER VII 172. MELTING D-R PELLETS The mathematical model described in Chapter V is utilized to determine the temperature distribution, the change of chemical composition, the volume of gases evolved,
University of Wollongong Research Online Australian Institute for Innovative Materials - Papers Australian Institute for Innovative Materials 2002 The effect of foamy slag in electric arc furnaces on electric
Induction Skull Melting Furnaces ISM The Process A B C D Induction Skull Melting ISM is a method of melting metals in a segmented, water-cooled copper vessel while under vacuum or controlled atmosphere
ALD Vacuum Technologies High Tech is our Business Vacuum Arc Remelting (VAR) Vacuum Arc Remelting Processes and Furnaces VAR Vacuum Arc Remelting (VAR) ALD is one of the leading suppliers of vacuum melting
Induction Technology REPORTS Inductive melting in steelworks by Mohamed Chaabet, Erwin Dötsch After the development of induction technology with inverter outputs of over 40 MW for crucible furnaces with
ISIJ International, Vol. 49 (009), No., pp. 668 67 Effect of Chromium on Nitrogen Solubility in Liquid Fe Alloys Containing 30 mass% Wan-Yi KIM, ) Chang-Oh LEE, ) Chul-Wook YUN ) and Jong-Jin PAK ) ) Formerly
Extracting and using metals Only the most unreactive metals such as gold and platinum are found as native metals. ores All the other metals we use are extracted from their ores by chemical processes. native
, pp. 413 418 Conversion of CO 2 Gas to CO Gas by the Utilization of Decarburization Reaction during Steelmaking Process Hiroyuki MATSUURA* and Fumitaka TSUKIHASHI Department of Advanced Materials Science,
1st semester 2015/2016 Arc welding SMAW CTU in Prague Faculty of Mechanical Engineering Ing. Petr Vondrouš, PhD., IWE SMAW welding Method no. standardized acc. ČSN EN ISO 4063 111 (Metal arc welding with
SPECIAL FOCUS REFRACTORIES A robot applies the colloidal silica bonded shotcrete material to a blast furnace. Better Refractories through NANOTECHNOLOGY by Michael Anderson, Senior Research Engineer, Magneco/
Development of a CaO-CaF 2 -slag system for high rare earth contents T. Müller; B. Friedrich IME Process Metallurgy and Metal Aachen University, Germany Prof. Dr.-Ing. Bernd Friedrich Source for Rare Earth:
INTERNATIONAL JOURNAL OF ENERGY RESEARCH Int. J. Energy Res., 22, 1049 1054 (1998) ENERGY ANALYSIS OF THE STEEL MAKING INDUSTRY MOUSA S. MOHSEN* AND BILAL A. AKASH Department of Mechanical & Industrial
Choosing the Right Technologies for Reverb Furnaces Russell Hewertson, Manager of Combustion Technology Choosing the Right Technologies for Reverb Furnaces Russell Hewertson, Manager of Combustion Technology
CHEMICAL AND STRUCTURAL CHARACTERIZATION OF DIFFERENT STEELMAKING DUSTS FROM STAINLESS STEEL PRODUCTION Frantisek Kukurugya 1)*, Tomáš Havlik 1), Antti Kekki 2) Olof Forsen 2) 1) Technical University of
Current Refractory Technology and Practices in the Steel Industry April 26, 2017 Rakesh K. Dhaka 2016 Steel Production in Numbers United States 4 th largest producer of steel in the world Source: World
Energy consumption, waste heat utilisation and pollution control in ferro alloy industry UMASHANKAR AGRAWAL Ferro Alloy Industry forms the backbone of the Iron Et Steel Industry in the World. Since energy
Dr. Joseph J Poveromo, Raw Materials & Ironmaking Global Consulting email@example.com DR Pellet Quality & MENA Applications Chemistry Considerations direct reduction processes: chemical
GENARAL INTRODUCTION TO METALLURGY :Std: XI-CHEMISTRY 1. What is matrix? The ore is generally associated with rock impurities like clay, sand etc. called gangue or matrix 2. What is mineral? The natural
CLASS: X NCERT (CBSE) SCIENCE: Chemistry Page: 1 Question 1: Compare the properties of a typical metal and a non-metal on the basis of the following. Fill in Column A, B. Properties A Metal B Non- metal
Steel Industry Technology Roadmap Barriers and Pathways for Yield Improvements by Energetics, Inc. for the American Iron and Steel Institute October 7, 2003 Table of Contents Executive Summary...ii 1 Modeling,
4th Slag Valorisation Symposium, 15-17 April 2015 Conditioning of Lead and Zinc Slags in Pilot Scale SAF for further Utilization Frank Kaußen, Jörn Böhlke, Christoph Kemper, Bernd Friedrich IME Process
STUDY ON SLAG RESISTANCE OF REFRACTORIES IN SUBMERGED ARC FURNACES MELTING FERRONICKEL Dong HU 1 Pei-Xiao LIU 2 Shao-Jun CHU 1 1 School of Metallurgical and Ecological Engineering, University of Science
4 Shielded Metal Arc Welding* * Abbreviated MMA (Manual metal arc welding). American designation: shielded metal arc welding (SMAW). Shielded metal arc welding (SMAW) is an AW process that uses a consumable
Non-Ferrous-Metallurgy in Aachen -Short Department Presentation B. Friedrich IME Process Metallurgy and Metal, RWTH Aachen University Prof. Dr.-Ing. Dr. h.c. Bernd Friedrich Our business education in non-ferrous